Chocks, Chocking and CHOCKFAST速 - Marine Chock Installation Presented by ITW Philadelphia Resins
Presentation Outline Basic Chocking Procedure Special Chocking Situations Some Chocking “Do’s & Don’ts” For More Information
Basic Chocking Procedure How to Chock a Marine Engine Step-by-Step
1. Determine Chock Volume ď€´Before the chocking job starts, develop a
Chocking Plan. ď€´Determine the total volume of all chocks including the overpour areas and subtracting the volume taken up by the bolts.
Order Chockfast Early Be sure to have at least 10% more Chockfast Orange than required in case of spills, leaks, etc. 3.4 kg (7.5 lbs) = 1966 cm3 (120 in3) 6.8 kg (15 lbs) = 4261 cm3 (260 in3)
2. Gather Materials Supplied by ITW PRC – Chockfast Orange – Open-cell Foam – Release Agent – Jiffy Mixing Blades – Non-melt Grease – Strip Caulking / Putty – PRT-51 Solvent
Supplied by Shipyard – 1/2” Drill Motor – Metal Dams – Safety Glasses – Disposable Vinyl Gloves – Surface Thermometer – Foam-backed Tape
3. Pre-condition the Chockfast Pre-condition the Chockfast Resin and hardener by storing it at 20oC to 25oC (68oF to 77oF) for at least 12 hours before use to ensure the epoxy will mix well and pour easily.
4. Clean Thoroughly Clean all surfaces of oil, grease, millscale, paint, and rust so that Chockfast makes complete contact with the foundation and bedplate.
It is also very important to remove all burrs and welding slag.
5. Insert Foam Dam Insert flexible damming along the back and on either side of the chock. Open-cell foam is best but neoprene can also be used.
Open-cell foam allows air to escape through it.
Insert Foam Dam A wood stick is a good tool for inserting foam. Be careful not to tear the foam. The foam should fit tightly between the steel to prevent the Chockfast from leaking.
A 6 mm (1/4 inch) press fit on the foam work best on soft foam.
6. Trim Ends of Foam Check to ensure that the damming is not twisted and is firmly in place. Cut off the protruding ends 25 mm (1 inch) from the engine bed plate.
7. Spray With Release Agent Only a very light spray is needed. The steel should NOT be wet with Release Agent.
8. Prepare to Plug The Bolt Hole Prepare to plug hole with either a greased bolt, an Armaflex tubing covered bolt, a greased wooden plug or a wooden dowel covered with foam tubing.
Bolt covered with grease
Foam or tape wrapped bolt
Grease covered wood dowel
Foam covered wood dowel
Always use non-melt grease.
9. Insert Plug/Bolt into the Hole The plug or bolt must prevent the Chockfast from leaking out from around the bolt hole. If using a bolt, install the nut hand-tight only.
10. Install the Front Dam Create a front dam by tack welding a 4 - 6 mm thick flat bar or angle iron, 12 to 18 mm from the bedplate. Seal the flat bar with putty or caulking. The front dam MUST be made of metal. The flat bar must be high enough to allow the Chockfast to be filled a minimum of 15 mm higher than the bottom of the bedplate.
11. Seal the Chock Mold Insert a piece of foam damming material at the front corners to prevent the Chockfast from overflowing. The foam can be press-fit into place or glued using contact cement.
Using putty, caulking or Silicone, seal all potential leak points.
12. Spray the Front Dam
Spray Release Agent on the inside of the front dam. Also spray Release Agent on top of the steel all around the front dam to make clean up easier.
13. Final Check Inspect all dams to ensure they are complete and well sealed. Measure the temperature of the steel and check the thickness of the chocks. Only when everything is ready should the Chockfast be brought out of storage and taken to the job site. If the steel temperature is below 13oC (55oF), use heaters to raise the temperature of the steel above 21oC (70oF) after the Chockfast has gelled for 24 hours.
14. Determine Required Hardener Using the Hardener Ratio Guide determine the correct amount of hardener to add to the resin.
Example: 20oC steel + 57 mm chock thickness = 1/2 Hardener Reduction
15. Squeeze Hardener into Resin Put on rubber gloves and eye protection. Puncture the paper seal under the bottle cap on the hardener. Turn the bottle of Hardener upside down and squeeze the amount of hardener called for in the Hardener Ratio Guide into the resin. Full Reduction = Squeeze in all BUT this amount of hardener 3/4 Reduction = Squeeze in all BUT this amount of hardener 1/2 Reduction = Squeeze in all BUT this amount of hardener 1/4 Reduction = Squeeze in all BUT this amount of hardener NO Reduction = Use ALL of the hardener
16. Mix the Resin & Hardener
Mix for 3 minutes.
Use a Jiffy Mixing blade or similar type mixing blade and a variable speed drill motor. Hold the can of Chockfast securely between your feet. Place the mixing blade all the way into the Chockfast and keep the blade submerged, traversing the can. Start mixing very slowly. Make sure the bottom of the can is scoured. Gradually increase the speed of the mixing blade but do not exceed 300 RPM.
17. Pour Chockfast
Pour Chockfast slowly, in a thin stream, from a height of about 300 mm (12 inches). A thin stream of Chockfast will force the air bubbles out of the mixture.
Pouring Chockfast Pour the Chockfast into the lowest corner of the overpour area. Pour it slowly and steadily into this one corner only. DO NOT scrape residue from the bottom or sides of the can.
18. Fill Chock Molds Fill the overpour area until the top of the Chockfast is at least 12 mm (Â˝ inch) above the bottom of the engine bed plate. Continually check for leaks. They can appear at any time. Do not leave until the chocks are hard.
19. Curing Allow the Chockfast to fully cure. The time required to cure depends on the steel temperature. 48 Hours
13oC - 18oC (55oF - 65oF)
19oC - 21oC (66oF - 70oF)
Above 21oC (70oF)
20. Clean Up
Wait until the Chockfast has completely cured before removing the outer metal dam. Gently pry it away from the Chockfast. Bevel the outside edge of the Chockfast removing the sharp edge using a grinder or sanding disc.
21. Back Out All Jacking Screws Remove all Jacking Screws or back them out 4 turns. If screws are removed, fill holes.
22. Torque Down Bolts First, back out all jacking bolts and remove all alignment devices. Then torque down all mounting bolts per engine manufacturerâ€™s instructions or contact ITW Philadelphia Resins.
RT LL = Righty Tighty - Lefty Loosey
Special Chocking Situations and How to Handle Them
Creating a Fitted Bolt
Spray the bolt with Release Agent. Seal the bottom of the bolt so it will not leak. Center the bolt in the hole and make sure it has 1/8 to 3/8 inch clearance. Fill chock area with Chockfast up to top of the bolt hole.
Jacking Screws Whenever possible, do not pour Chockfast around a jacking screw. If a jacking screw does fall inside a chock, wrap it with foam-backed tape, cover with Armaflex pipe insulation or coat with non-melt grease
Chocking In Layers The Hardener Ratio Guide sometimes calls for making â€œLayered Poursâ€? of Chockfast because the Chockfast may overheat if poured in a single layer. Use Layer Keys to prevent the edges from curling between pours. Pour successive layers within 4 to 6 hours.
Chocking with Limited Access Chockfast Orange can be injected with a grease gun
The outer metal dam can be installed at an angle
Some Chocking Do’s & Don’ts How to be more successful
DO Fill Up the Overpour 12mm Minimum
DONâ€™T Chock Around a Corner
Do NOT pour Chockfast around a corner. It will always lead to cracking because the corner acts like a wedge.
DO Round All Corners & Edges
When creating the chock mold, it is a good idea to round all corners and edges that may protrude into the Chockfast. This lessens the chance of cracking.
DONâ€™T Make the Overpour Too Large
The Chockfast in the overpour area must remain cool and liquid to feed material back under the engine bed if needed. To do this, the overpour must be small and kept cool with a heavy metal front dam.
DO Top off All Chocks
Sometimes the inside edge of the overpour will be drawn down slightly. Do not be concerned about this. Just top off the overpour area with some more Chockfast.
DONâ€™T Remove the Dams Until the Chockfast Has Fully Cured
Wait until the Chockfast has cured completely before removing the front metal dam or you could break the chock.
DO Prepare for Leaks Have non-hardening putty on hand for sealing small leaks that may appear. It is also a good idea to spray all areas adjacent to a chock with Release Agent to make clean up easier.
DONâ€™T Add Heat to A Chock Until the Chockfast Has Gelled
DO Pour Alternate Chocks
If overheating the Chockfast is a concern, fill every other chock, wait until they are cool then fill the remainder of the chocks.
DONâ€™T Forget the Release Agent
DO Make Sure the Dams Will Not Move
Watch Out For MAN B&W Engines
For More Information Where to go for help
Technical Bulletins TB 692 General Guidelines for Designing
Marine Chocks TB 659 Physical Properties of Chockfast Orange TB 656 Physical Properties of Chockfast Gray
Published on Jun 27, 2012
Published on Jun 27, 2012
- Marine Chock Installation - Presented by ITW Philadelphia Resins Presentation Outline Basic Chocking Procedure Special Chocking Situat...